- Nano Express
- Open Access
Facile Solution Synthesis of Red Phosphorus Nanoparticles for Lithium Ion Battery Anodes
Nanoscale Research Letters volume 13, Article number: 356 (2018)
Red phosphorus (RP) has attracted extensive attention as an anodic material for lithium-ion batteries (LIBs) due to its high theoretical specific capacity of 2596 mA h g− 1 and earth abundance. However, the facile and large-scale preparation of the red phosphorus nanomaterials via a solution synthesis remains a challenge. Herein, we develop a simple and facile solution method to prepare red phosphorus nanoparticles (RP NPs). PCl3 readily reacts with HSiCl3 in the presence of amines at room temperature to produce amorphous RP NPs with sizes about 100–200 nm in high yields. When used as an anode for rechargeable lithium ion battery, the RP NP electrode exhibits good electrochemical performance with a reversible capacity of 1380 mA h g− 1 after 100 cycles at a current density of 100 mA g− 1, and Coulombic efficiencies reaching almost 100% for each cycle. The study shows that this solution synthesis is a facile and convenient approach for large-scale production of RP NP materials for use in high-performance Li-ion batteries.
It has been realized for a long time that fossil fuels are non-renewable, finite, and environmentally harmful. Rechargeable lithium ion batteries (LIBs) with high energy density and long cycle life have stimulated extensive research interest because of their potentials as efficient and cheap energy storage systems [1,2,3]. The increasing demands for low-cost lithium ion batteries (LIBs) with high energy density and long cycle life call for the development of novel electrode materials [4,5,6,7]. The traditional graphite anode, commonly used in lithium ion batteries, is limited with respect to its low capacities (372 mA h g− 1) [8, 9]. To address this problem or issue, a great deal of efforts have been devoted to explore and develop alternative anode materials with substantially improved capacity and Coulombic efficiencies [10,11,12,13,14,15,16,17]. Among a wide range of high capacity anode materials, phosphorus and its composites show potential applications due to its low cost, abundance and high theoretical specific capacity (≈ 2600 mA h g− 1) [18,19,20,21,22].
Phosphorus has three allotropes, white P, black P, and red P . White P is toxic and chemically unstable, and is not suitable for the application in LIBs. Black P has good thermodynamic stability and conductivity, but the complex preparation process limits its large-scale applications [24,25,26]. Among these three different allotropes, red P is the most promising candidate  for the next generation high-energy anodic materials because of its stability and abundance. However, red P is plagued by its poor electronic conductivity (10− 12 S m− 1) and drastic volume change (300%) during the lithiation-delithiation process when served as anodes for rechargeable LIBs [28, 29].
To circumvent these impediments, red P has been encapsulated in different types of carbon host materials [30,31,32,33,34,35,36] to substantially improve the electrochemical performance of red P anodes for LIBs. For instance, Li et al. significantly improved both lithium storage and sodium storage performance of red P by confining nanosized amorphous red P into a mesoporous carbon matrix (P@CMK-3) via vaporization-condensation-conversion process . Ruan et al. designed a new strategy to embed red P particles into a cross-link-structural carbon film (P-C film) for use as a flexible binder-free anode in LIBs, in order to improve the electronic conductivity and accommodate the volume expansion . Nevertheless, the loading ratio of red P in the composite materials prepared by the vaporization–condensation method is typically low, which is unfavorable for the practical application [39, 40]. To this end, the use of nanoparticles or hollow nanostructures of red P prepared through size control and morphology engineering [41, 42] have been regarded as effective strategies to accommodate the large strain induced by the volume expansion and avoid material pulverization. For example, Chang et al. developed a large-scale synthesis of red phosphorus nanoparticles (RPNPs) through reduction of PI3 in iodobenzene by ethylene glycol in the presence of CTAB. The obtained RPNP electrodes exhibited a high-specific capacity, long cycling life, and excellent rate capability as anodes for LIBs . Moreover, Zhou et al. reported a wet solvothermal method to synthesize hollow red-phosphorous nanospheres with porous shells. The obtained hollow P nanosphere electrodes demonstrated high capacities and excellent long cycling performance due to the merits of the porous and hollow structures . Even though several literatures have reported the methods to the large-scale synthesis of red phosphorus, developing a high-yield and low-cost facile method to prepare the red phosphorus is still highly desirable. Particularly, the preparation of the red phosphorus nanomaterial via a solution synthesis remains a challenge.
Herein, we report a facile, rapid, and novel solution-based approach to synthesize RP NPs, employing room-temperature reaction of PCl3 with HSiCl3 in CH2Cl2 in the presence of amines. This new solution provides a cost-effective approach for massive production of red phosphorus nanoparticles for use in lithium ion batteries.
Trichlorosilane (HSiCl3) was purchased from TCI. n-Tripropylamine (Pr3N) was obtained from Aladdin. Phosphorus trichloride (PCl3) was purchased from Sinopharm Chemical Reagent Co. Ltd. Dichloromethane (CH2Cl2) was dried over CaH2 before use. All other chemical reagents were used as received without further purification.
Synthesis of Red Phosphorus Nanoparticles
In a typical preparation, 0.55 mL of Pr3N and 0.5 mL of HSiCl3 were added into 20 mL of anhydrous CH2Cl2. The formed colorless solution was magnetically stirred overnight at room temperature, during which the color turned into light yellow. And then 0.5 mL of PCl3 were added to the solution. Red phosphorus nanoparticles (RP NPs) were obtained in several seconds. The products were centrifuged, separated, and washed with anhydrous CH2Cl2, 1 M HF and distilled water to remove unreacted PCl3 and silica.
The electrochemical properties of red phosphorus nanoparticles as anode materials in LIBs were studied by using a 2032 coin cell assembly with lithium metal foils served as counter electrodes. The CR2032 cells were assembled in an argon-filled glovebox (both H2O and O2 < 0.1 ppm). The working electrode was prepared by mixing active material (RP NPs), conductive graphite and sodium carboxymethyl cellulose (CMC) in a weight ratio of 5:3:2 in deionized water to form a homogeneous slurry, which was then blade-deposited on a Cu foil. After drying at 80 °C for 12 h in vacuum, the foil was cut into disks of 14 mm in diameter. The total mass loading of active materials on the electrode was ~ 0.5 mg cm− 2. The electrolyte was 1.0 M LiPF6 in a mixture of 1:1 (v/v) ethylene carbonate/diethyl carbonate (Shenzhen Kejingstar Technology Ltd., China). The charge-discharge profiles of the half-cells were recorded using a Neware battery testing device (Shenzhen, China) at a constant current mode.
Powder X-ray diffraction (PXRD) was carried on a Bruker D8 X-ray diffractometer with a Cu Kα radiation (λ = 1.5418 Å). Scanning electron microscopy (SEM) images and energy dispersive spectroscopy (EDS) spectra (silicon wafers as the substrate) were obtained on a Hitachi field-emission scanning electron microscope (S-4800). Transmission electron microscopy (TEM) and high-resolution (HR) TEM were carried out with a JEM-2100 equipment (Japan). N2 adsorption isotherms were collected at 77 K (Micromeritics ASAP 2020 analyzer) after vacuum degassing of the sample at 100 °C for 10 h. Raman spectroscopy (LabRAM Aramis, Horiba, equipped with 633 nm laser) was used to investigate the structure of RP NPs. X ray photoelectron spectroscopy (XPS) measurements were recorded with a PHI 5000 VersaProbe. Thermo gravimetric (TG) analyses were conducted on a simultaneous STA449F3 (Netzche) thermal analyzer under flowing N2. The I-V curves of RP NPs were measured using cryogenic probe station Biologic VMP3 instrument (CRX-4K, Lake Shore, USA). Cyclic voltammetry (CV) tests were performed on a CHI650d electrochemical station (Shanghai Chenhua Instruments Inc., China).
Results and Discussion
Synthesis and Characterization of RPNPs
The red phosphorus nanoparticles (denoted as RP NPs) were synthesized via a facile solution method, which is depicted in Scheme 1. We found that phosphorus trichloride (PCl3) readily reacted with premixed HSiCl3 and tripropylamine (Pr3N) in CH2Cl2 at room temperature to produce orange powders in several seconds. The solution color changed to orange very rapidly when mixing a solution of HSiCl3–Pr3N–CH2Cl2 with PCl3, indicating the formation of RP NPs (Additional file 1: Figure S1). We postulated that PCl3 were reduced by subvalent oligosilane chlorides to form the phosphorus nanoparticles. The oligosilane chlorides were formed by the reaction of HSiCl3 with tripropylamine (Pr3N) in CH2Cl2 as results of disproportionation reaction of HSiCl3 in the presence of amine catalysts [45,46,47]. It is noted that the preformed oligosilane intermediates were essential for the occurrence of the reaction. Without amines (Pr3N), the reaction of HSiCl3 with PCl3 could not take place at room temperature. Similarly, the Pr3N could not react with PCl3 to produce RP NPs at room temperature. The yield of RP NPs, based on the amount of P atoms in PCl3, was approximately 38%, which is much higher than the reported literature . Furthermore, this solution-phase approach utilizes relatively low cost PCl3 instead of PI3 in iodobenzene, which could be more economically and easily scaled up to obtain large amounts of RP NPs. The color of the RPNPs was light orange, differing from the deep red color of commercial RP (Additional file 1: Figure S2).
PXRD analysis showed that the product was red phosphorus. As shown in Fig. 1a, the three broadened diffraction peaks at 13–16°, 25–38°, and 47–65°, consistent with the XRD pattern of commercial RP reported in the literature [21, 36]. SEM images show that the majority of RP NPs synthesized exhibited irregular-spherical shape with sizes about 100–200 nm in diameter. The corresponding SAED pattern of RP NPs (inset image of Fig. 2b) revealed that RP NPs were amorphous structure. Raman spectra of RP NPs presented three puckered peaks between 300 and 500 cm− 1, which is consistent with the Raman spectrum of commercial RP reported in the literature . The three peaks can be well assigned to the bond bending modes (B1 fundamental mode), bond bending vibrations (A1 symmetric stretch motion), and stretching vibrations (E1 degenerate mode) of amorphous red P (Fig. 1b). The thermal gravimetric analysis (TGA) of RPNPs in Fig. 3a shows a sharp weight loss between 380 and 430 °C under a nitrogen atmosphere owing to the sublimation, whereas commercial RP shows a sharp weight loss between 450 and 500 °C. The observed depression of sublimation temperature of RP NPs may result from high surface-to-volume ratios of nanoparticles [43, 48]. To quantitatively obtain the information of surface area, N2 sorption measurements (Fig. 3b) were conducted. The results revealed the Brunauer–Emmett–Teller (BET) surface area of RP NPs was about 37 m2 g− 1, which is much larger than that of the commercial RP.
In order to further characterize the structures, compositions, and chemical states of the prepared RP NPs, energy-dispersive X-ray spectroscopy (EDS) and X-ray photoelectron spectroscopy (XPS) measurements were carried out (Fig. 4). The EDS spectra shows that RP NPs are almost completely composed of elemental phosphorus. XPS survey spectrum (Fig. 4b) further confirms that P is the dominant element. The main peak in P 2p spectrum of XPS could be deconvoluted into two peaks at 129.74 and 130.74 eV, which correspond to the 2p3/2 and 2p1/2 of P in P–P bond, respectively, according to the previous literature [49, 50]. Moreover, a weak peak at 133.50 eV could be assigned to the P–O bond which was possibly formed through surface oxidation during air exposure. Therefore, the above results indicate the prepared nanoparticles are amorphous red P. In addition, the current-voltage (I-V) curves of RP NPs have been measured, as shown in Additional file 1: Figure S3. The conductivity of the RPNPs is about 1.7 × 10− 7 S m− 1 (0–2 V), which is 105 times higher than commercial RP (10− 12 S m− 1).
The electrochemical performance of the RP NPs as anode materials in LIBs was tested in CR2032 coin cells using a lithium metal foil as the counter electrode within the operating voltages of 0.01 to 2.5 V. Figure 5a depicts typical CV curves of the RP NPs at a scanning rate of 0.1 mV s− 1. There is a broad peak in the first lithiation cycle, which is ascribed to the activation process of inserting Li ions into phosphorus. A couple of redox peaks located at 0.5–0.75 V and 1.0–1.25 V are attributed to the lithiation of P and the delithiation of P–Li alloys [32, 51, 52] respectively. The deviation between the first and the subsequent cathodic curves implies irreversible capacity loss, which could be ascribed to the formation of the solid electrolyte interface (SEI) as well as to the occurrence of side reactions on the electrode surfaces, such as side reactions of defect sites, surface oxygen, and water impurities [36, 37, 53], a commonly observed behavior for LIB anodes. Figure 5b shows the typical discharge-charge voltage profiles of the RP NPs electrode for the first 3 cycles at a current density of 0.1 A g− 1. The apparent short discharge and charge voltage plateaus at around 0.7 V and 1.1 V are due to the lithiation and de-lithiation of RP NPs components, respectively, which agree well with the CV results. The electrode delivered a specific discharge and charge capacities of 2818 and 1641 mA h g− 1, respectively, for the first cycle, giving a first Coulombic efficiency of 58.2%. The decreased charge capacity could be attributed to the irreversible formation of the SEI membrane. It is noted that the Coulombic efficiency of RP NPs then quickly increased to 100% after the second cycle. The RP NPs exhibited an obvious capacity decay in the first 3 cycles. The irreversible capacity in the first few discharge-charge steps resulted from the decomposition of the electrolyte, which caused the formation of SEI on the electrode surface and the consumption of Li-ion. Moreover, the nanoparticles possess a high surface area in contact with the electrolyte solution, which would result in more side reactions, lowering the initial Coulombic efficiency in the first cycle .
The typical rate and long-term cycling stability performance of the RP NPs electrode are shown in Fig. 5c, d, respectively. RPNPs delivered the specific charge capacities of 1801, 1430, 1245, 1227, 1184, and 871 mA h g− 1 at the rates of 0.1, 0.2, 0.3, 0.5, and 1 A g− 1, respectively. The electrode showed good rate reversibility, with the specific discharge capacity recovered to the initial value when the current density returned to 0.1 A g− 1 after cycling at high current densities. The RP NPs finally maintained a high reversible discharge capacity of 1380 mA h g− 1, i.e., the retention of 89.1%, after 100 cycles with Coulombic efficiencies close to 100% throughout the measurements. Compared to commercial RP (Fig. 5e), RP NPs showed much improved long-term cycling stability.
In summary, we developed a new facile solution-phase approach to synthesis red phosphorus nanoparticles through the reaction of PCl3 and HSiCl3 in the presence of amines under the ambient environment. The RP NPs exhibited much better electrochemical performance with high reversible capacity and long-term cycling stability than commercial RP when served as anodes for rechargeable lithium ion battery. The RP NPs electrodes maintained a high reversible discharge capacity of 1380 mA h g− 1 (retention of 89.1%) after 100 cycles, with a Coulombic efficiency close to 100% for each cycle. This simple preparation method paves the way for cost-effective production of RP NPs as high-performance anodes for lithium-ion battery industry.
- CH2Cl2 :
Energy dispersive spectroscopy
- HSiCl3 :
- PCl3 :
Powder X-ray diffraction
- RP NPs:
Red phosphorus nanoparticles
Scanning electron microscopy
Transmission electron microscopy
X-ray photoelectron spectroscopy
Etacheri V, Marom R, Elazari R, Salitra G, Aurbach D (2011) Challenges in the development of advanced Li-ion batteries: a review. Energy Environ Sci 4(9):3243–3262
Goriparti S, Miele E, De Angelis F, Di Fabrizio E, Proietti Zaccaria R, Capiglia C (2011) Review on recent progress of nanostructured anode materials for Li-ion batteries. J Power Sources 257:421–443
Ellis BL, Lee KT, Nazar LF (2010) Positive electrode materials for Li-ion and Li-batteries. Chem Mater 2(3):691–714
Tarascon JM, Armand M (2001) Issues and challenges facing rechargeable lithium batteries. Nature 414:359–367
Bruce PG, Scrosati B, Tarascon JM (2008) Nanomaterials for rechargeable lithium batteries. Angew Chem Int Ed 47(16):2930–2946
Feng K, Li M, Liu W, Kashkooli AG, Xiao X, Cai M, Chen Z (2018) Silicon-based anodes for lithium-ion batteries: from fundamentals to practical applications. Small 14(1):1702737–1702770
Gonzalez AF, Yang NH, Liu RS (2017) Silicon anode design for lithium-ion batteries: progress and perspectives. J Phys Chem C 121(50):27775–27787
Kaskhedikar NA, Maier J (2009) Lithium storage in carbon nanostructures. Adv Mater 21(25–26):2664–2680
Mao Y, Duan H, Xu B, Zhang L, Hu Y, Zhao C, Wang Z, Chen L, Yang Y (2012) Lithium storage in nitrogen-rich mesoporous carbon materials. Energy Environ Sci 5(7):7950–7955
Kumai Y, Kadoura H, Sudo E, Iwaki M, Okamoto H, Sugiyama Y, Nakano H (2011) Si–C composite anode of layered polysilane (Si6H6) and sucrose for lithium ion rechargeable batteries. J Mater Chem 21(32):11941–11946
Ge M, Rong J, Fang X, Zhang A, Lu Y, Zhou C (2013) Scalable preparation of porous silicon nanoparticles and their application for lithium-ion battery anodes. Nano Res 6(3):174–181
Jia H, Gao P, Yang J, Wang J, Nuli Y, Yang Z (2011) Novel three-dimensional mesoporous silicon for high power lithium-ion battery anode material. Adv Energy Mater 1(6):1036–1039
Luo J, Liu J, Zeng Z, Ng CF, Ma L, Zhang H, Lin J, Shen Z, Fan HJ (2013) Three-dimensional graphene foam supported Fe3O4 lithium battery anodes with long cycle life and high rate capability. Nano Lett 13(12):6136–6143
Jing M, Zhou M, Li G, Chen Z, Xu W, Chen X, Hou Z (2017) Graphene-embedded Co3O4 rose-spheres for enhanced performance in lithium ion batteries. ACS Appl Mater Interfaces 9(11):9662–9668
Lu B, Ma B, Deng X, Li W, Wu Z, Shu H, Wang X (2017) Cornlike ordered mesoporous silicon particles modified by nitrogen-doped carbon layer for the application of Li-Ion battery. ACS Appl Mater Interfaces 9(38):32829–32839
Lv G, Zhu B, Li X, Chen C, Li J, Jin Y, Hu X, Zhu J (2017) Simultaneous perforation and doping of Si nanoparticles for lithium-ion battery anode. ACS Appl Mater Interfaces 9(51):44452–44457
Ma Q, Wang W, Zeng P, Fang Z (2017) Amorphous Ge/C composite sponges: synthesis and application in a high-rate anode for lithium ion batteries. Langmuir 33(9):2141–2147
Sun J, Zheng G, Lee HW, Liu N, Wang H, Yao H, Yang W, Cui Y (2014) Formation of stable phosphorus-carbon bond for enhanced performance in black phosphorus nanoparticle-graphite composite battery anodes. Nano Lett 14(8):4573–4580
Qian J, Wu X, Cao Y, Ai X, Yang H (2013) High capacity and rate capability of amorphous phosphorus for sodium ion batteries. Angew Chem Int Ed 125(17):4731–4734
Huang S, Cheong LZ, Wang D, Shen C (2017) Nanostructured phosphorus doped silicon/graphite composite as anode for high-performance lithium-ion batteries. ACS Appl Mater Interfaces 9(28):23672–23678
Kim Y, Park Y, Choi A, Choi NS, Kim J, Lee J, Ryu JH, Oh SM, Lee KT (2013) An amorphous red phosphorus/carbon composite as a promising anode material for sodium ion batteries. Adv Mater 25(22):3045–3049
Gao H, Zhou T, Zheng Y, Liu Y, Chen J, Liu H, Guo Z (2016) Integrated carbon/red phosphorus/graphene aerogel 3D architecture via advanced vapor-redistribution for high-energy sodium-ion batteries. Adv Energy Mater 6(21):1601037–1601044
Park CM, Sohn HJ (2007) Black phosphorus and its composite for lithium rechargeable batteries. Adv Mater 19(18):2465–2468
Zhang Y, Zheng Y, Rui K, Hng HH, Hippalgaonkar K, Xu J, Sun W, Zhu J, Yan Q, Huang W (2017) 2D black phosphorus for energy storage and thermoelectric applications. Small 13:1700661–1700681
Li QF, Duan CG, Wan XG, Kuo JL (2015) Theoretical prediction of anode materials in li-ion batteries on layered black and blue phosphorus. J Phys Chem C 119(16):8662–8670
Liu H, Du Y, Deng Y, Ye D (2015) Semiconducting black phosphorus: synthesis, transport properties and electronic applications. Chem Soc Rev 44:2732–2743
Zhou J, Jiang Z, Niu S, Zhu S, Zhou J, Zhu Y, Liang J, Han D, Xu K, Zhu L, Liu X, Wang G, Qian Y (2018) Self-standing hierarchical P/CNTs@rGO with unprecedented capacity and stability for lithium and sodium storage. Chem 4(2):372–385
Zaug JM, Soper AK, Clark SM (2008) Pressure-dependent structures of amorphous red phosphorus and the origin of the first sharp diffraction peaks. Nature Mater 7(11):890–899
Yabuuchi N, Matsuura Y, Ishikawa T, Kuze S, Son JY, Cui YT, Oji H, Komaba S (2014) Phosphorus electrodes in sodium cells: small volume expansion by sodiation and the surface-stabilization mechanism in aprotic solvent. Chem Electro Chem 1(3):580–589
Zhu Y, Wen Y, Fan X, Gao T, Han F, Luo C, Liou SC, Wang C (2015) Red phosphorus–single-walled carbon nanotube composite as a superior anode for sodium ion batteries. ACS Nano 9(3):3254–3264
Sun J, Lee HW, Pasta M, Sun Y, Liu W, Li Y, Lee HR, Liu N, Cui Y (2016) Carbothermic reduction synthesis of red phosphorus-filled 3D carbon material as a high-capacity anode for sodium ion batteries. Energy Storage Mater 4:130–136
Yuan D, Cheng J, Qu G, Li X, Ni W, Wang B, Liu H (2016) Amorphous red phosphorous embedded in carbon nanotubes scaffold as promising anode materials for lithium-ion batteries. J Power Sources 301:131–137
Li W, Hu S, Luo X, Li Z, Sun X, Li M, Liu F, Yu Y (2017) Confined amorphous red phosphorus in MOF-derived N-doped microporous carbon as a superior anode for sodium-ion battery. Adv Mater 29(16):1605820–1605828
Song J, Yu Z, Gordin ML, Li X, Peng H, Wang D (2015) Advanced sodium ion battery anode constructed via chemical bonding between phosphorus, carbon nanotube, and cross-linked polymer binder. ACS Nano 9(12):11933–11941
Yu Z, Song J, Gordin ML, Yi R, Tang D, Wang D (2015) Phosphorus-graphene nanosheet hybrids as lithium-ion anode with exceptional high-temperature cycling stability. Adv Sci 2(1–2):1400020–1400027
Li WJ, Chou SL, Wang JZ, Liu HK, Dou SX (2013) Simply mixed commercial red phosphorus and carbon nanotube composite with exceptionally reversible sodium-ion storage. Nano Lett 13(11):5480–5484
Li W, Yang Z, Li M, Jiang Y, Wei X, Zhong X, Gu L, Yu Y (2016) Amorphous red phosphorus embedded in highly ordered mesoporous carbon with superior lithium and sodium storage capacity. Nano Lett 16(3):1546–1553
Ruan J, Yuan T, Pang Y, Xu X, Yang J, Hu W, Zhong C, Ma ZF, Bi X, Zheng S (2017) Red phosphorus-embedded cross-link-structural carbon films as flexible anodes for highly reversible li-ion storage. ACS Appl Mater Interfaces 9(41):36261–36268
Marino C, Debenedetti A, Fraisse B, Favier F, Monconduit L (2011) Activated-phosphorus as new electrode material for li-ion batteries. Electrochem Commun 13(4):346–349
Wang L, He X, Li J, Sun W, Gao J, Guo J, Jiang C (2012) Nano-structured phosphorus composite as high-capacity anode materials for lithium batteries. Angew Chem Int Ed 51(36):9034–9037
Zhang Y, Rui X, Tang Y, Liu Y, Wei J, Chen S, Leow WR, Li W, Liu Y, Deng J, Ma B, Yan Q, Chen X (2016) Wet-chemical processing of phosphorus composite nanosheets for high-rate and high-capacity lithium-ion batteries. Adv Energy Mater 6(10):1502409–1502418
Winchester RA, Whitby M, Shaffer MS (2009) Synthesis of pure phosphorus nanostructures. Angew Chem Int Ed 48(20):3616–3621
Chang WC, Tseng KW, Tuan HY (2017) Solution synthesis of iodine-doped red phosphorus nanoparticles for lithium-ion battery anodes. Nano Lett 17(2):1240–1247
Zhou J, Liu X, Cai W, Zhu Y, Liang J, Zhang K, Lan Y, Jiang Z, Wang G, Qian Y (2017) Wet-chemical synthesis of hollow red-phosphorus nanospheres with porous shells as anodes for high-performance lithium-ion and sodium-ion batteries. Adv Mater 29(29):1700214–1700221
Tillmann J, Wender JH, Bahr U, Bolte M, Lerner HW, Holthausen MC, Wagner M (2015) One-step synthesis of a silafullerane with an endohedral chloride ion. Angew Chem Int Ed 54(18):5429–5433
Choi SB, Kim BK, Boudjouk P, Grier DD (2001) Amine-promoted disproportionation and redistribution of trichlorosilane: formation of tetradecachlorocyclohexasilane dianion. J Am Chem Soc 123(33):8117–8118
Tillmann J, Meyer L, Schweizer JI, Bolte M, Lerner HW, Wagner M, Holthausen MC (2014) Chloride-induced aufbau of perchlorinated cyclohexasilanes from Si2Cl6: a mechanistic scenario. Chem Eur J 20(30):9234–9239
Qi WH, Wang MP (2004) Size and shape dependent melting temperature of metallic nanoparticles. Mater Chem Phys 88(2–3):280–284
Li WJ, Chou SL, Wang JZ, Liu HK, Dou SX (2016) Significant enhancement of the cycling performance and rate capability of the P/C composite via chemical bonding (P-C). J Mater Chem A 4(2):505–511
Song J, Yu Z, Gordin ML, Hu S, Yi R, Tang D, Walter T, Regula M, Choi D, Li X, Manivannan A, Wang D (2014) Chemically bonded phosphorus/graphene hybrid as a high performance anode for sodium-ion batteries. Nano Lett 14(11):6329–6335
Qian J, Qiao D, Ai X, Cao Y, Yang H (2012) Reversible 3-li storage reactions of amorphous phosphorus as high capacity and cycling-stable anodes for li-ion batteries. Chem Commun 48(71):8931–8933
Yuan T, Ruan J, Peng C, Sun H, Pang Y, Yang J, Ma ZF, Zheng S (2018) 3D red phosphorus/sheared CNT sponge for high performance lithium-ion battery anodes. Energy Storage Mater 13:267–273
Wang B, Li X, Zhang X, Luo B, Jin M, Liang M, Dayeh SA, Picraux ST, Zhi L (2013) Adaptable silicon–carbon nanocables sandwiched between reduced graphene oxide sheets as lithium ion battery anodes. ACS Nano 7(2):1437–1445
Sun L, Wang F, Su T, Du H (2017) Room-temperature solution synthesis of mesoporous silicon for lithium ion battery anodes. ACS Appl Mater Interfaces 9(46):40386–40393
This work was supported by the National Natural Science Foundation of China (21471075).
Availability of Data and Materials
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Figure S1. The reaction process of RPNPs via the solution synthesis. Figure S2. Optical images of RPNPs and commercial RP powders. Figure S3. I-V curves of RPNPs. Figure S4. SEM images of commercial RP. (DOCX 631 kb)
About this article
Cite this article
Wang, F., Zi, W., Zhao, B.X. et al. Facile Solution Synthesis of Red Phosphorus Nanoparticles for Lithium Ion Battery Anodes. Nanoscale Res Lett 13, 356 (2018). https://doi.org/10.1186/s11671-018-2770-4
- Red phosphorous
- Solution method
- Lithium ion battery
- Anode material